Room Temperature Quantum Spin Hall Insulators with a Buckled Square Lattice Wei Luo† and Hongjun Xiang*,†,‡ †

Key Laboratory of Computational Physical Sciences (Ministry of Education), State Key Laboratory of Surface Physics, and Department of Physics, and ‡Collaborative Innovation Center of Advanced Microstructures, Fudan University, Shanghai 200433, P. R. China S Supporting Information *

ABSTRACT: Two-dimensional (2D) topological insulators (TIs), also known as quantum spin Hall (QSH) insulators, are excellent candidates for coherent spin transport related applications because the edge states of 2D TIs are robust against nonmagnetic impurities since the only available backscattering channel is forbidden. Currently, most known 2D TIs are based on a hexagonal (speciﬁcally, honeycomb) lattice. Here, we propose that there exists the quantum spin Hall eﬀect (QSHE) in a buckled square lattice. Through performing global structure optimization, we predict a new three-layer quasi-2D (Q2D) structure, which has the lowest energy among all structures with the thickness less than 6.0 Å for the BiF system. It is identiﬁed to be a Q2D TI with a large band gap (0.69 eV). The electronic states of the Q2D BiF system near the Fermi level are mainly contributed by the middle Bi square lattice, which are sandwiched by two inert BiF2 layers. This is beneﬁcial since the interaction between a substrate and the Q2D material may not change the topological properties of the system, as we demonstrate in the case of the NaF substrate. Finally, we come up with a new tight-binding model for a two-orbital system with the buckled square lattice to explain the low-energy physics of the Q2D BiF material. Our study not only predicts a QSH insulator for realistic room temperature applications but also provides a new lattice system for engineering topological states such as quantum anomalous Hall eﬀect. KEYWORDS: Quantum spin Hall eﬀect, topological insulator, square lattice, ﬁrst-principles calculations, structure prediction, two-dimensional material

T

opological insulators (TIs),1−7 as a new class of quantum materials, hold great potential for applications in quantum information, spintronics, ﬁeld eﬀect transistors, and thermoelectrics.8−14 The most interesting character of TIs is the presence of robust topological Dirac surface states in threedimensional (3D) TIs or helical edge states in two-dimensional (2D) TIs with spin locked to momentum as protected by timereversal symmetry. For coherent nondissipative spin transport related applications, 2D TIs are better than 3D TIs as the electrons at the edges of 2D TIs can only move along two directions with opposite spins and thus free from backscattering caused by nonmagnetic defects, whereas the surface states of 3D TIs are only free from exact 180°-backscattering and suﬀer from scattering of other angles. Currently, quantum spin Hall eﬀect (QSHE) was experimentally observed only at very low temperatures.6,7 There is great interest in searching for room temperature (RT) 2D TIs. Among all predicted or synthesized 2D TIs, the hexagonal honeycomb lattice is the most common motif. For instance, graphene was predicted to be the ﬁrst 2D topological insulator (TI).15 However, QSHE in graphene may only be observed at an extremely low temperature due to its tiny band gap (about 8 × 10−4 meV16) opened by spin−orbit coupling (SOC) eﬀect. © XXXX American Chemical Society

Subsequently, silicene with a buckled honeycomb lattice was predicted to be a 2D TI with a larger band gap (about 1.55 meV) due to its stronger intrinsic SOC eﬀect and buckling eﬀect.10 Unfortunately, the band gap is still too small for RT application, and free-standing silicene or silicene grown on an insulating substrate have not been obtained experimentally. Wang et al. predicted that a 2D organometallic triphenyl-metal compound with the hexagonal lattice is a new organic TI with a band gap of about 8.6 meV.14 Very recently, Song et al. proposed that quasi-2D (Q2D) honeycomb Bi halide systems are huge-band gap (up to 1.08 eV) TIs. These giant-gaps are entirely due to the result of strong on-site SOC being related to the px and py orbitals of the Bi atoms around the two valley K and K′ of the honeycomb lattice.17 Experiments are awaited to check the stability of 2D honeycomb Bi halides. We note that Wu et al. studied systematically the physics of the honeycomb lattice with px and py orbitals.18−20 Although the presence of the Dirac band structure makes the honeycomb lattice the most common platform for engineering the topological states, a large Received: February 1, 2015 Revised: March 13, 2015

A

DOI: 10.1021/acs.nanolett.5b00418 Nano Lett. XXXX, XXX, XXX−XXX

Letter

Nano Letters

indicate that Bi4F4 is thermally stable at least up to 500 K (see Supplementary Figure S2). The local density approximation (LDA) band structure of Bi4F4 is shown in the left panel of Figure 1b. We can see a Dirac cone at the Fermi level close to the Y point. The detailed analysis shows that the bands around the Fermi level are mainly contributed by px and py orbitals of the middle Bi layer of Bi4F4. The pz orbitals of the middle Bi layer lie at around −1.5 and 2.0 eV with respect to the Fermi level (see Supplementary Figure S3). We note that the electron−phonon coupling removes the Dirac cone near one X point and the other cone lying between Γ and M point due to the presence of the in-plane distortion of the middle Bi layer. After including the SOC eﬀect, the band gap opens at the Dirac point (see Figure 1b). The whole system has an indirect band gap of 0.37 eV with the conduction band minimum (CBM) near (0, 0.5). Since LDA usually underestimates the band gap, we adopt the more reliable hybrid functional HSE0624 to ﬁnd that the indirect band gap is 0.69 eV (see Supplementary Figure S4). It is large enough for RT applications. Because Bi4F4 has an inversion symmetry, we can calculate the topological Z2 invariant by counting the parity of the occupied states25 and ﬁnd that Bi4F4 is a 2D TI (Z2 = 1). For realistic applications, the Q2D Bi4F4 material should lie on a substrate, or Bi4F4 can be directly grown on a substrate. We ﬁnd that the lattice constant of Bi4F4 is very close to that of the insulating substrate NaF. The lattice mismatch between NaF and Bi4F4 is about 2.0%. We suggest that the [001] NaF surface can be a good substrate for Bi4F4 (see Supplementary Figure S5a). Our band structure calculation shows that the whole system has a band gap and that states near the Fermi level are mostly contributed by Bi px and py orbitals of Bi4F4 (see Supplementary Figure S5b). We ﬁnd that Bi4F4 on the NaF substrate is still a TI. In order to conﬁrm this, we gradually decrease the distance between Bi4F4 and the substrate NaF and ﬁnd that the band gap does not close. In other words, the interaction between the insulating NaF substrate and Bi4F4 is weak so that the topological nontrivial electronic properties of Bi4F4 remain intact. It is noted that the two inert outer layers make the topological properties of Bi4F4 more insensitive to the substrate, diﬀerent from the cases of silicene and bilayer Bi. We also check the robustness of the TI electronic structure of Bi4F4 with respect to an epitaxial strain. Our LDA+SOC calculations show that the indirect band gap of Bi4F4 increases with strain and that there is a ﬁnite gap even when a 5% compressive strain is present (see Figure 2). Note that the quasi-particle band gap should be larger since LDA underestimates the band gap. Electronic Structures of a Simple Model System Bi2F2. The main physics of Bi4F4 can be understood by considering a simpler system. As already mentioned above, Bi4F4 is composed by two BiF2 layers and a middle Bi layer. The BiF2 layer is inert since their electronic states are far from the Fermi level. The chemical bonding in the outer BiF2 layer can be analyzed as follows. In a BiF2 layer, each Bi atom is surrounded by four F atoms and forms a covalent bond with one Bi atom from the middle Bi layer; each F atom forms bonds with two Bi atoms of the BiF2 layer. Among the ﬁve valence electrons (6s26p3) of a Bi atom, two electrons transfer to the neighboring F atoms, one electron is used to form a pz−pz σ bond with the Bi atom from the middle layer, and the remaining two electrons occupy the lone-pair 6s orbital. For a Bi atom in the middle Bi layer, one electron is used to form the pz−pz σ bond with the Bi atom of the BiF2 layer, two electrons occupy the lone-pair 6s orbital, and the remaining two low-energy electrons will occupy the px

gap 2D TI suitable for realistic RT applications remains to be synthesized experimentally. A nature question then arises: Does QSHE exist in other simple lattices? Addressing this question successfully will not only enrich our understanding of topological phenomena but also pave new ways for designing topological materials for realistic applications. In this work, we suggest that QSHE can occur in the buckled square lattice. With our newly developed global optimization approach, we predict that a new quasi-2D (Q2D) material (i.e., Bi4F4) with a distorted square lattice of Bi is much more stable than the previously proposed honeycomb BiF structure.17 This Bi4F4 system is identiﬁed to be a room temperature TI with a large band gap (0.69 eV). A new tight-binding (TB) model for the buckled square lattice with two orbitals per site is proposed to understand the origin of the topological nontrivial electronic properties of Bi4F4. Results and Discussion. Geometrical and Electronic Structures of the Q2D Bi4F4 Material. As we discussed above, the hypothetical Q2D honeycomb BiF compound is found to be a large-gap TI.17 However, it may not be the lowest energy structure. With our newly developed global optimization approach for predicting Q2D materials (see Methods),21 we perform an extensive search to ﬁnd more stable Q2D BiF structures. Our calculations show that the Q2D BiF structure (shown in Figure 1a) has the lowest energy among all

Figure 1. Geometrical and electronic structures of Bi4F4. (a) Top and side views of Bi4F4. The top and bottom layers are inert BiF2 layers. The square lattice of the middle Bi layer is slightly distorted. (b) LDA band structures of Bi4F4 without (left panel) and with (right panel) SOC. The contribution from px and py orbitals of the middle Bi layer is highlighted.

structures with the thickness less than 6.0 Å. Since the unit cell contains four formula units of BiF, we refer to this structure as Bi4F4. Instead of the hexagonal lattice, Bi4F4 takes a distorted square lattice with two slightly diﬀerent lateral lattice constants (4.520 and 4.527 Å). The total energy of this structure is lower than that of 2D honeycomb BiF17 by about 0.42 eV/atom. The formation energy of Bi4F4 is calculated to be 1.62 eV/atom with respect to bulk Bi and ﬂuoride molecule, indicating no phase separation behavior. Our Q2D Bi4F4 structure can be seen as a stacking of three layers: A bismuth layer with the distorted buckled square lattice is sandwiched between two BiF2 layers. The computed phonon frequencies22,23 (see Supplementary Figure S1) indicate that Bi 4 F 4 is dynamically stable. Furthermore, ﬁrst-principles molecular dynamics simulations B

DOI: 10.1021/acs.nanolett.5b00418 Nano Lett. XXXX, XXX, XXX−XXX

Letter

Nano Letters

the lattice is divided into two sublattices [A (top) and B (bottom)]. This square lattice has an in-plane lattice spacing d, and for simplicity, we assume d = 1 in the following discussion. We can see that the lateral mirror symmetry is broken due to the buckling, but the system still has spatial inversion symmetry at the bond centers between the nearest-neighbor (NN) A and B sites. At each lattice point, there are two orbitals px and py. The number of electrons in a primitive cell is four, i.e., halfﬁlled case. The total eﬀective low-energy Hamiltonian contains three parts:

Figure 2. Band gap of Bi4F4 as a function of epitaxial strain from the LDA+SOC calculations. The indirect band gap increases with strain Δ (Δ = (a − a0)/a0, where a and a0 is the lateral lattice constants of the strained and unstrained systems, respectively). Even a large compressive strain (about −5%) can not destroy the nontrivial topological properties, indicating the robust TI behavior in Bi4F4. Note that LDA underestimates the band gap.

H = Ht + Hso + H1

with

∑

Ht =

[t ppσ(ci+, xsci ± x ̂, xs + ci+, ysci ± y ̂, ys)

i∈A ,s

+ t ppπ(ci+, xsci ± y ̂, xs + ci+, ysci ± x ̂, ys)] + H . c .

and py orbitals. Therefore, we can adopt a simple model structure Bi2F2 (see Figure 3) to understand the low-energy

Hso =

⎛ iλ + ⎞ iλ ⎜− ci , x ↑ci , y ↑ + ci+, x ↓ci , y ↓⎟ + H . c . ⎝ 2 ⎠ 2 i ∈ {A , B}

∑

and H1 =

∑ i ∈ A , d ̂, α , s

t deff̂, αsci++ d ̂, α s ci , αs + H . c . ̅ ̅

where ci,αs destructs a particle with spin s (↑ or ↓ along the z axis) on the α (px or py) orbital at the site i; x̂ ≡ (1,0) and ŷ ≡ (0,1) represent the unit vectors in the x and y directions, respectively. The ﬁrst term Ht represents the usual NN hopping term between the p orbitals with the Slater−Koster interaction parameters tppσ (>0) and tppπ (0) represents the ̅ ̅ magnitude of the eﬀective hopping. Physically, this eﬀective hopping may originate from a two-step process. As an example, we show how this works for the case of t xeff̂, y ↑ in Figure 4c. Although the basis of our low-energy Hamiltonian only contains px and py orbitals, there are high-lying pz orbitals in reality. In the ﬁrst step, a spin-up electron on the py orbital of the A sublattice hops into the spin-down pz orbital due to the on-site SOC. Then, this electron transfers to the spin-down px orbital of the NN B-site, which is possible due to the presence of the buckling. Note that the second step is forbidden in a planar square lattice, which makes the eﬀective NN hopping term vanish there. Overall, the eﬀective NN hopping term is a ﬁrst-order SOC eﬀect with teff ∝ λ. This two-step process is diﬀerent from the cases of systems with the honeycomb lattice. In graphene and silicene, the relevant orbital is pz, and there is eﬀective next-NN hopping due to the second-order16 or ﬁrstorder SOC10 eﬀect, respectively. However, the on-site SOC was found to be responsible for the band gap opening in C

DOI: 10.1021/acs.nanolett.5b00418 Nano Lett. XXXX, XXX, XXX−XXX

Letter

Nano Letters

Figure 4. Description and electronic properties of our new TB model for a buckled square lattice. (a) Schematic illustration of the buckled square lattice. The red and blue balls represent sublattices A (top) and B (bottom), respectively. One space inversion center in the middle of NN A and B sites is denoted by “i”. (b) Band structures of the buckled square lattice in the cases of the usual hopping (Ht, left panel), usual hopping and on-site SOC (Ht + Hso, middle panel), and all three terms (Ht + Hso + H1, the right panel), respectively. The parities of states at Γ are marked. (c) Illustration of how a ﬁrst order SOC eﬀect induces the eﬀective NN hopping for the case of t xeff̂, y ↑. (d) The phase diagram of the TB model for a positive teff. The olive region represents TI. The red dot denotes the case of Bi2F2. (e) Band gap as a function of the eﬀective NN hopping teff when ﬁxing other parameters.

honeycomb Bi halides with the low-energy px and py orbitals.17 In the following, we will show that the eﬀective NN hopping H1 plays a key role in realizing the TI state. We now discuss the electronic structure of our newly proposed model. First, we only consider the usual hopping term Ht. A typical band structure with tppσ = 1.0 and tppπ = −0.2 is shown in the left panel of Figure 4b. We can see that there are two kinds of Dirac cones at the Fermi level; one locates at X point, and another lies between Γ and M. These Dirac cones can be seen as a result of the Brillouin zone folding since Ht does not break the translation symmetry along x̂ and ŷ. We ﬁnd that all four degenerate occupied bands at Γ have even parity, while there are two occupied even-parity bands and two occupied odd-parity bands for the other three time-reversalinvariant k-points (two X and one M). The fact that the states with even parity have lower energy than those with odd parity at Γ can be easily understood by the orbital interaction picture (see Supplementary Figure S7). Second, we add the on-site SOC term Hso. The band structure in the case of λ = 1.2 is shown in the middle panel of Figure 4b. Obviously, the Dirac cones are kept although their positions are shifted. Therefore, the on-site SOC eﬀect can not open a band gap in the buckled square lattices, in contrast to the case of honeycomb Bi halides.17 Some bands split due to the on-site SOC interaction. In particular, the 4-fold degenerate occupied bands at Γ split into two 2-fold degenerate states whose parities remain even. Finally, we ﬁnd that the eﬀective NN hopping H1 can open a band gap at the Dirac points, as shown in the right panel of Figure 4b for the case of teff = 0.2. The magnitude of the band gap is almost proportional to teff when ﬁxing other parameters (see Figure 4e). Note that there is no gap if we switch oﬀ the on-site SOC term. An important ﬁnding is that all four occupied states at Γ have even parity, while the number of occupied states with even parity is the same as that with odd

parity for X and M. According to the parity criteria,25 the system is a 2D TI (Z2 = 1). Therefore, we ﬁnd that the eﬀective NN hopping due to SOC is indispensable for the occurrence of the QSHE. We now investigate the dependence of the ground state on the parameters of the model Hamiltonian in details. As we discussed above, the system is not a TI whenever teff = 0. Now, we consider the case of teff > 0. We ﬁnd that the system becomes a trivial insulator when the on-site SOC is too strong. This can be understood as follows. Since the parities of the occupied states at X and M do not depend on λ, we can focus on the eigenstates at Γ. By solving exactly the full model Hamiltonian at Γ, we obtain four 2-fold degenerate states: EI = −λ/2 − 2(tppσ + tppπ), EII = λ/2 − 2(tppσ + tppπ), EIII = −λ/2 + 2(tppσ + tppπ), and EIV = λ/2 + 2(tppσ + tppπ). States I and II have even parity, while states III and IV have odd parity. Interestingly, these eigenvalues are independent of teff. Since λ > 0 and usually tppσ + tppπ > 0, state I with the lowest energy is always occupied, while state IV with the highest energy is always empty. Whether state II has a lower energy than state III depends on the relative magnitude of sign of λ/4 and tppσ + tppπ. When the on-site SOC is weak, i.e., λ/4 < tppσ + tppπ, state II with even parity is occupied and the system is in a TI state. On the contrary, state III with odd parity is occupied and the system is a trivial insulator. The phase diagram in the case of teff > 0 is shown in Figure 4d. Noted that our model is diﬀerent from that of the FeSe system proposed by Hao et al.27 Their model is intended to describe the interactions between d orbitals, the band gap induced by the SOC is small, and the appearance of the topological phase needs the help of a substrate. We ﬁnd that the band structure of Bi2F2 is very similar to that of our new TB Hamiltonian (compare Figure 4b and Figure 3). It is anticipated that the low-energy physics of Bi2F2 can be D

DOI: 10.1021/acs.nanolett.5b00418 Nano Lett. XXXX, XXX, XXX−XXX

Letter

Nano Letters

bismuth and ﬂuoride is ﬁxed to 1:1, and the chemical formula ranges from Bi1F1 to Bi8F8. We consider six diﬀerent initial thickness (between 1 and 6 Å) for each system. In addition, we repeat each calculation twice in order to ensure the results reliable.

described by our model. In order to prove this point, we obtain the low-energy eﬀective Hamiltonian by using the maximally localized Wannier function (MLWF).28−30 We choose px and py orbitals as the projection functions for each Bi atom. The band structure near the Fermi level is reproduced rather well by the MLWF Hamiltonian (see the right panel of Figure 3, denoted by blue lines). With the MLWF basis, we can obtain the parameters of our above TB model Hamiltonian: tppσ = 1.34 eV, tppπ = −0.26 eV, λ = 1.40 eV, and teff = 0.13 eV. Other interactions such as further neighbor hopping are found to be much weaker. Therefore, Bi2F2 and thus Bi4F4 can be well described by our model for the buckled square lattice. Conclusions. Using the new particle swarm optimization (PSO) approach adapted for the Q2D systems, we predict that the most stable Q2D structure with the thickness less than 6 Å is a three-layer structure (i.e., Bi4F4) for BiF, in which the middle Bi layer takes a distorted square lattice. We ﬁnd that Bi4F4 is a RT TI with a band gap of 0.69 eV. The TI state in Bi4F4 is robust with respect to the interaction with substrate and epitaxial strain. In order to understand its topological electronic structures, we propose a TB model for the buckled square lattice with two orbitals (i.e., px and py) per site. We show that the band inversion is due to the chemical hybridization between the px and py orbitals. Diﬀerent from the cases of 2D systems (graphene, silicene, and honeycomb Bi halides) with a honeycomb lattice, a newly discovered eﬀective NN hopping term due to the SOC is crucial for the gap opening of a Dirac cone. Bonding analysis and MLWF calculations suggest that the low-energy electronic structure of Bi4F4 can be described rather well by the new TB model. In this work, we not only predict a RT quantum spin Hall insulator with a distorted square lattice for realistic spintronic applications but also provide a new basic TB model for investigating topological states in the simple square lattice. Methods. DFT Calculations. In our work, density functional theory (DFT) method is used for structural relaxation and electronic structure calculation. The ion−electron interaction is treated by the projector augmented-wave31 technique as implemented in the Vienna ab initio simulation package.32 The exchange-correlation potential is treated by LDA.33,34 For structural relaxation, all the atoms are allowed to relax until atomic forces are smaller than 0.01 eV/Å. The HSE06 functional is adopted to compute the accurate band gap.24 PSO Algorithm for Q2D Systems. To obtain the most stable Q2D structure of BiF, we adopt our newly developed global optimization PSO approach for predicting Q2D materials.21 In our implementation, we generate random Q2D structures with the thickness along the c-axis smaller than a given thickness. For each Q2D structure, we ﬁrst randomly select a layer group instead of a planar space group.35 The lateral lattice parameters and atomic positions are then randomly generated but conﬁned within the chosen layer group symmetry. Subsequently, local optimization including the atomic coordinates and lateral lattice parameters is performed for each of the initial structures. In the next generation, a certain number of new structures (the best 60% of the population size) are generated by PSO.36 The other structures are generated randomly, which is critical to increase the structure diversity. When we obtain the new Q2D structure by the PSO operation or random generation, we make sure that the thickness of the Q2D structure is smaller than the given thickness. In our simulation for the BiF system, we set the population size to 30 and the number of generations to 20. The ratio of

■

ASSOCIATED CONTENT

S Supporting Information *

Figures displaying phonon dispersions, thermal stability, band structures, geometrical and electronic structures, and schematic illustration wave functions. This material is available free of charge via the Internet at http://pubs.acs.org.

■

AUTHOR INFORMATION

Corresponding Author

*E-mail: [email protected]. Notes

The authors declare no competing ﬁnancial interest.

■

ACKNOWLEDGMENTS The work was supported by NSFC, the Special Funds for Major State Basic Research, FANEDD, NCET-10-0351, Research Program of Shanghai Municipality and MOE, Program for Professor of Special Appointment (Eastern Scholar), and Fok Ying Tung Education Foundation.

■

REFERENCES

(1) Hasan, M. Z.; Kane, C. L. Rev. Mod. Phys. 2010, 82, 3045. (2) Qi, X. L.; Zhang, S. C. Rev. Mod. Phys. 2011, 83, 1057. (3) Yan, B. H.; Zhang, S.-C. Rep. Prog. Phys. 2012, 75, 096501. (4) Qian, X.; Liu, J.; Fu, L.; Li, J. Science 2014, 346, 1344. (5) Bernevig, B. A.; Hughes, T. L.; Zhang, S. C. Science 2006, 314, 1757. (6) König, M.; Wiedmann, S.; Brüne, C.; Roth, A.; Buhmann, H.; Molenkamp, L. W.; Qi, X. L.; Zhang, S. C. Science 2007, 318, 766. (7) Knez, I.; Du, R. R.; Sullivan, G. Phys. Rev. Lett. 2011, 107, 136603. (8) Weng, H. M.; Dai, X.; Fang, Z. Phys. Rev. X 2014, 4, 011002. (9) Kane, C. L.; Mele, E. J. Phys. Rev. Lett. 2005, 95, 146802. (10) Liu, C. C.; Feng, W. X.; Yao, Y. G. Phys. Rev. Lett. 2011, 107, 076802. (11) Murakami, S. Phys. Rev. Lett. 2006, 97, 236805. (12) Chuang, F. C.; Yao, L. Z.; Huang, Z. Q.; Liu, Y. T.; Hsu, C. H.; Das, T.; Lin, H.; Bansil, A. Nano Lett. 2014, 14, 2505. (13) Xu, Y.; Yan, B. H.; Zhang, H. J.; Wang, J.; Xu, G.; Tang, P. Z.; Duan, W. H.; Zhang, S. C. Phys. Rev. Lett. 2013, 111, 136804. (14) Wang, Z. F.; Liu, Z.; Liu, F. Nat. Commun. 2012, 4, 1471. (15) Kane, C. L.; Mele, E. J. Phys. Rev. Lett. 2005, 95, 226801. (16) Yao, Y. G.; Ye, F.; Qi, X. L.; Zhang, S. C.; Fang, Z. Phys. Rev. B 2007, 75, 041401. (17) Song, Z. G.; Liu, C. C.; Yang, J. B.; Han, J. Z.; Fu, B. T.; Ye, M.; Yang, Y. C.; Niu, Q.; Lu, J.; Yao, Y. G. NPG Asia Mater. 2014, 6, e147. (18) Wu, C. J.; Bergman, D.; Balents, L.; Sarma, S. D. Phys. Rev. Lett. 2007, 99, 070401. (19) Wu, C. J. Phys. Rev. Lett. 2008, 101, 186807. (20) Zhang, G. F.; Li, Y.; Wu, C. J. Phys. Rev. B 2014, 90, 075114. (21) Luo, W.; Ma, Y. M.; Gong, X. G.; Xiang, H. J. J. Am. Chem. Soc. 2014, 136, 15992. (22) Parlinski, K.; Li, Z. Q.; Kawazoe, Y. Phys. Rev. Lett. 1997, 78, 4063. (23) Togo, A.; Oba, F.; Tanaka, I. Phys. Rev. B 2008, 78, 134106. (24) Heyd, J.; Scuseria, J. E. J. Chem. Phys. 2003, 118, 8207. (25) Fu, L.; Kane, C. L. Phys. Rev. B 2007, 76, 045302. (26) Slater, J. C.; Koster, G. F. Phys. Rev. 1954, 94, 1498. (27) Hao, N. N.; Hu, J. P. Phys. Rev. X 2014, 4, 031053. (28) Mostofi, A. A.; Jonathan, R. Y.; Lee, Y. S.; Souza, I.; Vanderbilt, D.; Marzari, N. Comput. Phys. Commun. 2008, 178, 685. E

DOI: 10.1021/acs.nanolett.5b00418 Nano Lett. XXXX, XXX, XXX−XXX

Letter

Nano Letters (29) Marzari, N.; Vanderbilt, D. Phys. Rev. B 1997, 56, 12847. (30) Souza, I.; Marzari, N.; Vanderbilt, D. Phys. Rev. B 2001, 65, 035109. (31) Blöchl, P. E. Phys. Rev. B 1994, 50, 17953. (32) Kresse, G.; Hafner, J. Phys. Rev. B 1994, 49, 14251. (33) Perdew, J. P.; Zunger, A. Phys. Rev. B 1981, 23, 5048. (34) Ceperkey, D. M.; Alder, B. J. Phys. Rev. Lett. 1980, 45, 566. (35) Luo, X. Y.; Yang, J. H.; Liu, H. Y.; Wu, X. J.; Wang, Y. C.; Ma, Y. M.; Wei, S. H.; Gong, X. G.; Xiang, H. J. J. Am. Chem. Soc. 2011, 133, 16285. (36) Wang, Y. C.; Lv, J.; Zhu, L.; Ma, Y. M. Phys. Rev. B 2010, 82, 094116.

F

DOI: 10.1021/acs.nanolett.5b00418 Nano Lett. XXXX, XXX, XXX−XXX